- 60 Views
- Uploaded on
- Presentation posted in: General

Interactive experimentation and thermodynamic modeling

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

Interactive experimentation and thermodynamic modeling

Weiping Gonga, Marcelle Gaune-Escardb, Zhanpeng Jina

aState Key Lab of Powder Metallurgy, Central South University,

Changsha, Hunan, P. R. China

bEcole polytechnique, Mecanique Energetique,

Technopole de Chateau-Gombert, Marseille, France.

The CODATA conference, Beijing, China, 2006

1. Introduction

2. Structural behavior and thermodynamic properties of SrZrO3

3. Thermodynamic modeling and experimentation of KBr-TbBr3 system

4. Summaries

- Phase diagram’s functions: blueprints or roadmap for materials design, development, processing and basic understanding
- visual representations of the state of a material: T, P, C

- The correlation between thermodynamics and phase equilibrium
- J. W. Gibbs
- Modern development: modeling and computer technology
phase equilibrium computer calculation possibility

- Crucial thermodynamic modeling in binary system
- can be extrapolated to multi-component systems
- Question: Can we believe the results of modeling?

- Two method to check the results of modeling
- Comparison between the calculated and measured data in literature is the most usually employed test (example one on SrZrO3)
- the best way is to couple interactive experimentation and modeling (example two on KBr-TbBr3)

- Two example were used to illustrate theses two methods
- Structure behavior and thermodynamic properties of SrZrO3
- KBr-TbBr3 Phase diagram and the decomposition of K3TbBr6

- Two different reviews about the structure behavior of SrZrO3 existed in literature
- One review: the room temperature structure of SrZrO3 was pseudo-cubic, and this pseudo-cubic structure did not undergo any phase transformation upon heating
- Second review: the room temperature structure of SrZrO3 was orthorhombic, and the orthorhombic perovskite SrZrO3 will transform through higher symmetries during heating, eventually to ideal cubic

- A series of thermodynamic data available in literature but great difference existed
- Different structure?
- Effect of impurities, minor departures from nominal stoichiometry, or changes in synthesis temperatures?

- How to identify and resolve the inconsistency between various kinds of experimental data?
- Basic tool: thermodynamic modeling
- complementary experimentation

- Experimental data evaluation and thermodynamic modeling
- Thermodynamic data and structural information evaluation, thus two optimization procedure were adopted
- One optimization procedure: don’t consider structure transformation
Thermodynamic modeling of SrZrO3:

GSrZrO3= a1+b1·T +c1·T ·lnT+d1·T 2+e1·T–1 (1)

- Second optimization procedure: consider structure transformation,
Thermodynamic modeling of SrZrO3:

similar equation as (1) to describe orthorhombic SrZrO3

pGSrZrO3 = oGSrZrO3 + ΔH1 - T · ΔS1 (2)

tGSrZrO3= pGSrZrO3 + ΔH2 - T · ΔS2 (3)

cGSrZrO3= tGSrZrO3 + ΔH3 - T · ΔS3 (4)

ΔH1,ΔS1,ΔH2,ΔS2,ΔH3,ΔS3are the corresponding enthalpies and entropies of the transformations

- One optimization procedure: don’t consider structure transformation

- Thermodynamic data and structural information evaluation, thus two optimization procedure were adopted

- Comparison between Experimental data and Thermodynamic calculation

Structure transformation and the corresponding enthalpy were detected by

thermodynamic modeling

- Prepare the samples
- Solid reaction to prepare SrZrO3: SrCO3 + ZrO2
- Heat-treated at 1150, 1000, 850 0C
- Air quenched or furnace-cooled

- XRD determination

- XRD curve: sample quenched from 1150 0C and furnace-cooled to room temperature show the cubic and orthorhombic structure, respectively.

The observed patterns from SrZrO3, showing the fundamental perovskite reflections. The patterns were recorded at 850, room temperature and 1150oC

- XRD curve results illustrate:
negative the pseudo-cubic SrZrO3 in room temperature,

confirm the structure transformation

it’s quite difficult to obtain the tetragonal SrZrO3 due to

the impurity, minor departures from nominal stoichiometry

- Thermodynamic modeling and experimentation benefit the structure behavior and thermodynamic properties investigation
- Thermodynamic modeling is based on the experimental information and can be used to identify and resolve the inconsistency between various kinds of experimental

Example 2: KBr-TbBr3 system

- Measured KBr-TbBr3 phase diagram byL. Rycerz et al

- Two eutectic reactions
- Three compounds
- K3TbBr3: a solid phase transition at 691 K, melt congruently at 983 K
- K2TbBr5: a solid phase transition at 658 K, melt incongruently at 725 K
- KTb2Br7: form from K2TbBr5 and TbBr3 at 694K, melt incongruently at 741 K

- Measured thermodynamic data byL. Rycerz and M. Gaune-Escard
- Heat capacity of K3TbBr6:thermal effect at about 691 and 983K
- Enthalpy of mixing of liquid at 1113 K: the minimum located at about 0.3 KBr suggested the existence of TbBr6-3

Thermodynamic modeling of KBr-TbBr3 system

- thermodynamic modeling of each phase
- Phase without composition range: G(T) function
- Compounds without thermodynamic data: Neumann-Kopp rule
K2TbBr5: A1+B1·T +2/3·GKBr(s)+1/3·GTbBr3(s)

KTb2Br7 : A2+B2·T +1/3·GKBr(s)+2/3·GTbBr3(s)

- K3TbBr6 with thermodynamic data and structural information
two equations were used to describe two forms of K3TbBr6

lGK3TbBr6= a1+b1·T +c1·T ·lnT+d1·T 2+e1·T–1

hGK3TbBr6= a2+b2·T +c2·T ·lnT+d2·T 2+e2·T–1

- Compounds without thermodynamic data: Neumann-Kopp rule
- Thermodynamic description of liquid phase:
- associated solution (K+)P (Br-, TbBr6-3, TbBr3)Qwas introduced to describe short-range order around K3TbBr6 composition

- Phase without composition range: G(T) function

- Thermodynamic calculation and comparison (Thermo-Calc software)
- Calculated phase diagram
- Good agreement
- Exception:
decomposition of K3TbBr6 at 593 K

- The detected thermo effect in the heat
capacity curve of K3TbBr6 at low temperature

- Assessed to be structure change
- Key experiments were conducted to
check the existence temperature range

of K3TbBr6

- Calculated phase diagram

Key experiments to check the existence temperature of K3TbBr6

- Prepare the samples
- DSC measurements between room temperature and 650 K with a rate of 1 K/min
- DSC heating and cooling curve:
thermal effect at about 593K

- Results:
K3TbBr6 KBr + K2TbBr5

at 593 K

- DSC heating and cooling curve:

DSC heating and cooling traces on K3TbBr6 compound

Conclusions

- Based on the measured data, each phase in KBr-TbBr3 system was thermodynamically modeling, KBr-TbBr3 phase diagram and thermodynamic properties were preliminarily calculated.
- Guided by the calculated phase diagram and thermodynamic properties, key experiments were carried out, then model of the relate phases were modified to explain the literature and the present measured experimental data.
- The finally obtained thermodynamic properties and phase diagram were more reasonable

Summaries

- Two examples, i.e. structure behavior of SrZrO3 and the phase diagram of KBr-TbBr3 system were provided to illustrate the interactive experimentation and thermodynamic modeling
- Thermodynamic calculation is based on the experimental data and can provide important information for materials experiments, thus guide materials design, development, processing and materials understanding.

Thank You !

Welcome to China !